x

请选择需要导出的字段：

ASTM D2837-2008

Standard Test Method for Obtaining Hydrostatic Design Basis for Thermoplastic Pipe Materials or Pressure Design Basis for Thermoplastic Pipe Products

适用范围：<p>The procedure for estimating long-term hydrostatic strength or pressure-strength is essentially an extrapolation with respect to time of a stress-time or pressure-time regression line based on data obtained in accordance with Test Method D 1598<astmref rid="a00002">. Stress or pressure-failure time plots are obtained for the selected temperature and environment: the extrapolation is made in such a manner that the long-term hydrostatic strength or pressure strengthis estimated for these conditions. </p> <p class="desc"> <span class="smallcap">Note</span> 38212;Test temperatures should preferably be selected from the following: 40<span class=''unicode''>x00B0;</span>C; 50<span class=''unicode''>x00B0;</span>C; 60<span class=''unicode''>x00B0;</span>C; 80<span class=''unicode''>x00B0;</span>C; 100<span class=''unicode''>x00B0;</span>C. It is strongly recommended that data also be generated at 23<span class=''unicode''>x00B0;</span>C for comparative purposes. </p> <p>The hydrostatic or pressure design basis is determined by considering the following items and evaluating them in accordance with 5.4. </p> <p>Long-term hydrostatic strength or hydrostatic pressure-strength at 100 000 h, </p> <p>Long-term hydrostatic strength or hydrostatic pressure-strength at 50 years, and </p> <p>Stress that will give 5 % expansion at 100 000 h. </p> <p>The intent is to make allowance for the basic stress-strain characteristics of the material, as they relate to time. </p> <p>Results obtained at one temperature cannot, with any certainty, be used to estimate values for other temperatures. Therefore, it is essential that hydrostatic or pressure design bases be determined for each specific kind and type of plastic compound and each temperature. Estimates of long-term strengths of materials can be made for a specific temperature provided that calculated values, based on experimental data, are available for temperatures both above and below the temperature of interest. </p> <p>Hydrostatic design stresses are obtained by multiplying the hydrostatic design basis values by a service (design) factor. </p> <p>Pressure ratings for pipe may be calculated from the hydrostatic design stress (HDS) value for the specific material used to make the pipe, and its dimensions using the equations in 3.1.11. </p> <p>4.5.1 Pressure ratings for multilayer pipe may be calculated by multiplying the pressure design basis (PDB) by the appropriate design factor (DF).</p><p id="s00002">1.1 This test method describes two essentially equivalent procedures: one for obtaining a long-term hydrostatic strength category based on stress, referred to herein as the hydrostatic design basis (HDB); and the other for obtaining a long-term hydrostatic strength category based on pressure, referred to herein as the pressure design basis (PDB). The HDB is based on the material''s long-term hydrostatic strength (LTHS),and the PDB is based on the product''s long-term hydrostatic pressure-strength (LTHS<sub>P</sub>). The HDB is a material property and is obtained by evaluating stress rupture data derived from testing pipe made from the subject material. The PDB is a product specific property that reflects not only the properties of the material(s) from which the product is made, but also the influence on product strength by product design, geometry, and dimensions and by the specific method of manufacture. The PDB is obtained by evaluating pressure rupture data. The LTHS is determined by analyzing stress versus time-to-rupture (that is, stress-rupture) test data that cover a testing period of not less than 10 000 h and that are derived from sustained pressure testing of pipe made from the subject material. The data are analyzed by linear regression to yield a best-fit log-stress versus log time-to-fail straight-line equation. Using this equation, the material''s mean strength at the 100 000-h intercept (LTHS) is determined by extrapolation. The resultant ......

实施日期： 2008-05-01

中标分类号： G33 - 化工 - 塑料型材

ICS分类号： 83.140.30 - 橡胶和塑料工业 - 塑料管、配件和阀门

标准组织： ASTM - 美国材料与试验协会标准

全文来源： WF

英文关键词： Circumferential expansion Design--piping systems Hydrostatic design basis (HDB) Polyethylene (PE) pipe Stress--plastics Thermoplastic pipe/tube/fittings Validation

语种： 汉语

页数： 16

替代关系：
该标准替代了如下标准：ASTM D2837-2004e1

知识产权声明 | 服务承诺 | 联系我们 | 客户服务 | 关于我们

网络出版服务许可证：(署)网出证(京)字第072号 药品医疗器械网络信息服务备案：(京)网药械信息备字（2023）第 00470 号 信息网络传播视听节目许可证 许可证号：0108284

万方数据标准管理系统V2.0 证书号:软著登字第11198474号

京ICP证：010071 京公网安备11010802020237号 京ICP备08100800号-1

客服电话：4000115888 客服邮箱：service@wanfangdata.com.cn 违法和不良信息举报电话：4000115888 举报邮箱：problem@wanfangdata.com.cn 举报专区：https://www.12377.cn

万方数据知识服务平台--国家科技支撑计划资助项目（编号：2006BAH03B01）©北京万方数据股份有限公司 万方数据电子出版社